*Research Article*

**Mechanical Properties Optimization of Friction Stir Welded**

**Lap Joints in Aluminium Alloy**

**Antonio Viscusi , Antonello Astarita , and Umberto Prisco**

*Department of Chemical, Materials and Production Engineering, University of Napoli Federico II, Piazzale Tecchio 80,*
*80125 Napoli, Italy*

Correspondence should be addressed to Umberto Prisco; umberto.prisco@unina.it

Received 7 November 2018; Revised 18 January 2019; Accepted 28 January 2019; Published 17 February 2019 Guest Editor: Dariusz Rozumek

Copyright © 2019 Antonio Viscusi et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

This work focuses on the inﬂuence of the rotational and travel speed on the strength of AA 2024 T3 friction stir welded lap joints. Tensile tests were carried out on minispecimens extracted from diﬀerent welding zones. A central composite design was applied to identify the relative importance of the variable factors’ eﬀects and their interaction on yield/ultimate strength and elongation for both the heat aﬀected-zone (HAZ) and nugget zone. Surface methods and gradient algorithms were used to optimize the yield strength of the joints. Shear and microhardness tests were executed to achieve a more complete mechanical characterization.

**1. Introduction**

The feasibility of replacing the riveting process with friction stir welding (FSW) technology in the assembly of fuselage skin-stiﬀener panels was the objective of several scientiﬁc papers in the last decades [1–6]. The potential of FSW to result in signiﬁcantly lower assembly times and manufacturing costs, yet higher productivity, cannot be overemphasized. However, commercial applications of this process require addressing issues such as strength analysis and design as well as optimizing the manufacturing process parameters for more reliable welds with minimum distor-tion [7, 8]. One of the many experimental strategies used to determine the process parameters as well as to optimize the process is deﬁned “by trial” and relies on the researcher’s technical and theoretical process knowledge [9]. This strategy consists of a sequential procedure wherein the value of just one parameter among the set of parameters identiﬁed in the previous experiment is varied. This speciﬁc parameter is the one that mostly inﬂuences the process response while keeping ﬁxed the level of the other parameters [10]. Such an approach has at least two disadvantages: it lacks objectivity in determining mathematical relations between process inputs and response variables and it also lacks eﬃciency and

accuracy in optimizing the surface response through trials [11]. Another experimental strategy is the “one factor per time approach,” wherein the researcher subsequently varies the levels of each factor within its range while keeping ﬁxed at the base level the other factors [12]. Obviously, this ap-proach lacks information about the factors’ interactions, but it enables estimating main factors’ eﬀects. In any event, the one factor per time approach is less accurate and less eﬃcient than the statistical approach [13]. Many studies of experi-mental strategies prove that the correct experiexperi-mental strategy for problems involving more than one factor and data points aﬀected by experimental errors must be taken from design of experiments (DOE) techniques if the aim is to remove objective results from experimental data [14]. These techniques allow maximum conclusive information to be drawn from minimum work, time, energy, money, or other limited resources. So, DOE aims to maximize information per run by choosing a reduced number of input sample points. Moreover, it enables developing a robust process, i.e., a process that minimizes the inﬂuence of noise variables [15]. Data organized by DOE allow the most powerful use of analysis of variances, since main factor and interaction ef-fects can be estimated to determine their signiﬁcance. An-other considerable advantage of using these techniques

Volume 2019, Article ID 3832873, 9 pages https://doi.org/10.1155/2019/3832873

involves combining DOE with response surface method-ologies (RSMs), more eﬃciently to evaluate the eﬀectiveness of investigative trade-oﬀs [16]. One of the most important advantages of using DOE techniques is extrapolation [17]. This property is signiﬁcant because it allows optimum prediction even if “optimum” lies outside the initial design range, and the number of runs must be reduced to achieve optimum. Good predictive properties allow DOE association with other complex mathematical methods without com-promising accuracy and assuring the method of steepest ascent. This method is a viable technique for sequentially moving toward the optimum response [18]. A compre-hensive recitation of additional advantages of these DOE techniques is beyond the scope of this paper. Several papers deal with the inﬂuence of process parameters on properties of FSW joints [19–22]; in particular, it was adopted a DOE to investigate such inﬂuence [23]. From the literature, it is also evident that the main process parameters that need to be investigated are the rotational speed and travel speed [24– 26]. In particular, it was proved that the inverse of travel speed measurements was better than travel speed to ﬁt experimental data [27]. Therefore, this study examined the strength of FSW aluminium alloy lap joints in two diﬀerent welding zones: HAZ and nugget zone. Aiming to test sep-arately the tensile strength of HAZ and nugget zone, minispecimens from both these zones were subjected to shear and microhardness tests. The process parameters optimization issue was approached using central factorial design, response surface methods, and gradient algorithms.

**2. Materials and Methods**

AA 2024 T3 sheets were used as the bottom and the top sheet of the lap joints. The nominal weight percent com-position (major alloying additions) of AA 2024 is 4.4% Cu, 1.5% Mg, 0.6% Mn, and the rest is aluminium. Sheets’ thickness is 1.27 mm. The ultimate tensile strength (UTS) of the AA 2024 T3 base metal is 475 MPa. As for the welding process parameters, the inverse of travel speed (TS−1) ranged from 0.155 to 0.533 s/mm and the rotational speed (RS) ranged from 950 to 2222.5 rpm. Plunge depth was ﬁxed to 2.11 mm, tilt angle to zero degree, and travel angle to one degree.

Nine diﬀerent TS−1-RS combinations were used for
obtaining 13 welds in this study; ﬁve combinations were
derived by 22factorial design with ﬁve centre points, and the
remaining four combinations were obtained by using the
steepest ascent algorithm. One tool conﬁguration equipped
with a pin consisting of a threaded frustum of the cone was
used; the lower and the upper diameters are 2.77 mm and
5.06 mm, respectively, with a length of 2.03 mm. The
shoulder diameter is 12.04 with a concavity of 7°_{. Two}
diﬀerent machines were used to perform FSW lap and
overlap joints with single pass. A controlled numerical
machine (CNM) was employed to perform the set of runs
concerned with the central factorial design featured by high
heat generation (hot runs); a vertical milling machine was
used to carry out the set of runs concerned with the steepest
algorithm featured by low heat generation (cold runs).

Both the top and bottom sheets, 152.40 mm long and
2.54 mm thick, were positioned as shown in Figure 1. Sheets
were degreased prior to welding using acetone as a cleaner.
After the FSW process, an optical specimen was taken out
from each run; microscope observations of the cross sections
were carried out to identify the exact position of the welding
zones. At the same time, the cross sections of the welds were
observed and analysed by image processing software to
identify the position of the hook defects and measure the
grain size. According to ASTM E 112, the grain size number
is determined by using the general intercept method. For this
purposes, standard metallographic polishing procedures
were used with modiﬁed Keller’s reagent. Thanks to the
aforementioned analyses, it was possible to remove three
minitensile specimens from both the nugget and
heat-aﬀected zones for each run by using a minimilling machine.
Minitensile testing was carried out by following design of
experiments. Figure 2 shows the minitensile specimen
drawing with its geometrical dimensions. It is worth to note
that smaller is the specimen higher are the mechanical
properties recorded; experimental results of minitensile
samples refer to local properties of the material which exceed
the global ones [28]. Each sample was pulled out from the lap
joints; then, it was reﬁned and polished on both sides by
*using abrasive papers of 30 µm and 12 µm removing *
ex-ceeding material and leading the thickness from 1 mm to
*0.50 mm. Abrasive papers of 9 µm and 3 µm were used to*
eliminate the surface scratches; ﬁnally, a diamond
*suspen-sion of 1 µm was used to create a like-mirror surface. The*
waiting time between the welding and the minitensile testing
was typically 150 h. The minitensile testing was performed
through a minitensile testing machine by imposing a strain
rate equal to 10−3s−1. The ultimate strength, the yield
strength, and the elongation of the weld were measured. The
last property was evaluated by using the Epsilon ONE optical
high-precision extensometer, which is a noncontact device
able to measure accurately the strain of this type of
mini-tensile specimen at the narrow section.

The mechanical characterization of the lap joints ob-tained by FSW technology also included shear testing and microhardness measurements. The strength of the lap joints loaded nominally in overlap shear was examined, even though in this case, 150 h elapsed before shear testing was carried out. All the specimens tested were 25.4 mm wide, 127 mm long, and 2.54 mm thick (Figure 3), manufactured using a shear machine, and ground on both sides by milling. Three specimens for each run were tested, and the failure loads were averaged. All overlap shear tests were performed using the same strain rate used in the tensile testing. The maximum loads (failure loads) were recorded for each specimen. Each weld was sectioned and polished so the hardness could be measured using a digital Vickers hardness tester. The centre of the welds was tested throughout the cross section with 1 mm spacing between data points; all welding zones down to the base material were involved.

As for the experiments design, the central composite design (CCD), able to ﬁt the response surface through a quadratic regression model, was used in this study. CCD contains an embedded factorial or fractional factorial design

with centre points that are augmented with a group of “star points.” The importance of the centre points is that they allow for a curvature estimation [29]. The CCD could be implemented more easily with a sequential procedure: ﬁrstly, a factorial design with centre points should be per-formed to estimate the signiﬁcance of the main factor eﬀects and interaction eﬀects, and above all to prove or to reject the presence of a curvature. Then, if the presence of the cur-vature is proved, the “star points” procedure can be per-formed. According to the aforementioned procedure, a 22 factorial design with ﬁve centre points and three repeated measurements was carried out to perform tensile testing for the nugget zone and for the heat-aﬀected zone. The ex-perimental table is summarized (Table 1).

To avoid systematic errors, the whole set of experiments has been randomized. To perform an ANOVA in every possible case, even in the case of heteroskedasticity of data (i.e., not constant variance), a weighted ANOVA was carried out [30]. Such analysis requires repeated measurements for each run. Experimental data of yield strength, ultimate strength, and elongation are analysed and plotted separately. MINITAB, one of the most common statistical software packages, was used to deﬁne the DOE table and to perform a weighted ANOVA as well as residuals analysis. Experiments included repeats of the response, whose measurements allowed variability analysis in response data through a weighted regression. Such a method is suitable for handling data with diﬀerent variances.

**3. Results and Discussion**

Experimental data of yield strength are shown in Table 2. An important point is that the column called WGTS_ADJ contains weights, i.e., an estimate of the reciprocal variance of the mean. These weights are due to the analysis of var-iability that is shown in Table 3. This analysis calculates and stores the standard deviations of the repeated responses detecting diﬀerences or dispersion eﬀects across factor settings. This analysis even allows weights to be stored to perform a weighted ANOVA.

This analysis shows that only two eﬀects could be
*considered signiﬁcant: rpm with a p value of 0.094 and the*
*inverse of the travel speed with a p value of 0.055; the *
in-teraction eﬀect seems not to be noticeable. Neither curvature
could be considered signiﬁcant. The weighted ANOVA
related to the experimental data of yield strength is shown in
Table 4. The regression model has been reduced by removing
the interaction eﬀect since a previous analysis proved its
*negligibility; in fact, the value of F related to the interaction*
*eﬀect is 0.09 corresponding to a p value of 0.782.*

*The analysis shows a curvature p value of 0.145 that*
*cannot be able to prove its presence and a main eﬀect p value*
of 0.040 that ensures a signiﬁcant inﬂuence; speciﬁcally, the
*pvalue related to rpm is 0.0045, and the p value related to*
TS−1is 0.0055. Both the values can be considered signiﬁcant.
Regression model coeﬃcients are estimated as shown in
Table 4. Aiming to prove the model adequacy, residuals
analysis was performed that is not here reported for the sake
of brevity. Such an analysis veriﬁed the hypothesis made on
the residuals; i.e., residuals can be assumed to be normally
127 mm

50.8 mm

25.4 mm

25.4 mm

Figure 3: Shear specimens drawing.

Table 1: Table data for two factorial designs with ﬁve centre points.

Runs order rpm s/mm
1 1377.5 0.267
7 2222.5 0.267
6 1377.5 0.533
5 2222.5 0.533
2 1800.0 0.400
3 1800.0 0.400
4 1800.0 0.400
9 1800.0 0.400
8 1800.0 0.400
Sheet interface
Tool rotation
Retrea
ting side
Weldin
g dir
ectio_{n}
Adva_{ncin}
g side
Weld zone

Figure 1: Schematic of friction stir welding.

7.6 mm
1.8 mm
1.1 mm
4.6 mm
*R0.76 mm*
*R0.25 mm*

Small tensile specimen dimensions (1 mm width)

distributed with null average and constant standard
de-viation. Moreover, the regression model ﬁts the data very
*well since the high p value related to the lack of ﬁt (0.782) is*
just a consequence of the interaction term omission.
Ex-perimental data of ultimate strength are shown in Table 5.
The analysis of variability related to the experimental data of
ultimate strength is shown in Table 6.

It can be seen that only two eﬀects could be considered
*signiﬁcant: rpm with a p value of 0.059 and the inverse of the*
*travel speed with a p value of 0.006; the interaction eﬀect*
seems not to be noticeable. Either curvature could be
considered signiﬁcant. The weighted ANOVA related to the
experimental data of ultimate strength is shown in Table 7.
The regression model presented has been reduced by

Table 4: Results of yield strength weighted analysis of variance. Estimated eﬀects and coeﬃcients for avg. Ys (coded units)

Term Eﬀect Coef. SE coef. *T* *p*

Constant — 346.718 3.953 87.71 0.0

rpm −15.948 −7.974 3.004 −2.65 0.0045

s/mm −17.026 −8.513 3.413 −2.49 0.0055

Ct Pt — 8.469 4.903 1.73 0.45

*S � 0.533470* *R*2�73.27% *R*2(adj) � 57.24%
Analysis of variance for avg. Ys (coded units)

Source DF Seq. SS Adj. SS Adj. MS *F* *p*

Main eﬀects 2 3.051 3.709 1.855 6.52 0.040 Curvature 1 0.849 0.850 0.850 2.98 0.145 Residual error 5 1.423 1.422 0.285 — — Lack of ﬁt 1 0.031 0.030 0.030 0.09 0.782 Pure error 4 1.393 1.392 0.348 — — Total 8 5.327 — — — —

Estimated coeﬃcients for avg. Ys using data in uncoded units

Term Coef.

Constant 406.30

rpm −0.019

s/mm −64.01

Ct Pt 8.47

Table 2: Yield strength experimental responses.

rpm s/mm Ys1 Ys2 Ys3 Ys4 Std. Ys Dim Avg. Ys WGTS_ADJ

1377.5 0.267 372 365 353 — 9.609 3 363.333 0.0390 2222.5 0.267 361 323 356 — 20.648 3 346.667 0.0084 1377.5 0.533 349 319 368 — 24.705 3 345.333 0.0059 2222.5 0.533 402 345 249 343 63.373 4 334.750 0.0011 1800.0 0.400 353 356 326 — 16.523 3 345.000 0.0063 1800.0 0.400 356 374 320 — 27.495 3 350.000 0.0063 1800.0 0.400 360 366 348 — 9.165 3 358.000 0.0063 1800.0 0.400 342 357 397 338 26.938 4 358.500 0.0084 1800.0 0.400 355 343 392 — 25.541 3 363.333 0.0063

Table 3: Results of yield strength analysis of variability. Regression estimated eﬀects and coeﬃcients for natural log of std. Ys ratio (coded units)

Term Eﬀect Eﬀect Coef. SE coef. *T* *p*

Constant — — 3.0796 0.1407 21.89 0.0

rpm 0.8733 2.395 0.4367 0.2118 2.06 0.094

s/mm 1.0527 2.865 0.5264 0.2118 2.49 0.055

rpm ∗ s/mm 0.1084 1.115 0.0542 0.2118 0.26 0.808

*R*2�72.04% *R*2(adj) � 55.26%
Analysis of variance for natural log of std. Ys

Source DF Seq. SS Adj. SS Adj. MS *F* *p*

Main eﬀects 2 6.319 5.900 2.950 5.981 0.047 2-Way interactions 1 0.032 0.032 0.032 0.070 0.808 Residual error 5 2.465 2.465 0.493 — — Curvature 1 0.130 0.130 0.130 0.222 0.661 Pure error 4 2.335 2.335 0.583 — — Total 8 8.816 — — — —

removing the interaction eﬀect since a previous analysis
*proved its negligibility. In fact, the value of F related to the*
*interaction eﬀect is 0.41 corresponding to a p value of 0.558.*
*The analysis shows a signiﬁcant curvature p value, whose*
*value is less than 0.001, a main eﬀect p value less than 0.001*
*ensuring a huge signiﬁcant inﬂuence; speciﬁcally, the p value*
*related to rpm is less than 0.001 and the p value related to*

TS−1is 0.001. Both the eﬀects can be considered very
sig-niﬁcant. Regression model coeﬃcients are estimated as
shown in Table 7. It was also performed a residuals analysis
that seems to verify the hypothesis made on the residuals, so
they can be assumed to be normally distributed with null
average and constant standard deviation. By the way, the
*regression model cannot ﬁt well the data, even if the p value*

Table 5: Ultimate strength experimental responses.

rpm s/mm Us1 Us2 Us3 Us4 Std. US Dim Avg. US WGTS_ADJ

1377.5 0.267 502.0 480.0 484.0 — 11.719 3 488.667 0.0324 2222.5 0.267 431.0 432.5 460.2 — 16.443 3 441.233 0.0081 1377.5 0.533 444.6 419.5 478.0 — 29.348 3 447.367 0.0026 2222.5 0.533 435.6 452.0 285.0 392 75.160 4 391.150 0.0008 1800.0 0.400 491.0 501.4 449.0 — 27.743 3 480.467 0.0046 1800.0 0.400 496.6 492.5 428.6 — 38.131 3 472.567 0.0046 1800.0 0.400 456.0 485.7 483.3 — 16.498 3 475.000 0.0046 1800.0 0.400 475.7 451.8 494.0 — 21.162 3 473.833 0.0046 1800.0 0.400 472.0 466.8 514.0 — 25.881 3 484.267 0.0046

Table 6: Results of ultimate strength analysis of variability. Regression estimated eﬀects and coeﬃcients for natural log of std. US ratio (coded units)

Term Eﬀect Eﬀect Coef. SE coef. *T* *p*

Constant — — 3.2266 0.0909 35.48 0.0

rpm 0.6428 1.902 0.3214 0.1317 2.44 0.059

s/mm 1.2221 3.394 0.6111 0.1317 6.64 0.006

rpm ∗ s/mm 0.3041 1.355 0.1520 0.1317 1.15 0.301

*R*2_{�}_{87.80%} * _{R}*2

_{(adj) � 80.48%}

Analysis of variance for natural log of std. US

Source DF Seq. SS Adj. SS Adj. MS *F* *p*

Main eﬀects 2 6.6109 5.8970 2.9485 15.46 0.007 2-Way interactions 1 0.2540 0.2540 0.2540 1.33 0.301 Residual error 5 0.9537 0.9537 0.1907 — — Curvature 1 0.0037 0.0037 0.0037 0.02 0.907 Pure error 4 0.9500 0.9500 0.2375 — — Total 8 7.8187 — — — —

Table 7: Results of ultimate strength weighted analysis of variance. Estimated eﬀects and coeﬃcients for avg. US (coded units)

Term Eﬀect Coef. SE coef. *T* *p*

Constant — 442.97 2.973 148.99 0.0

rpm −48.23 −24.12 1.860 −12.96 0.0

s/mm −43.49 −21.75 2.798 −7.77 0.001

Ct Pt — 34.26 3.629 9.44 0.0

*S � 0.3170* *R*2_{�}_{97.93%} * _{R}*2

_{(adj) � 96.68%}

Analysis of variance for avg. US (coded units)

Source DF Seq. SS Adj. SS Adj. MS *F* *p*

Main eﬀects 2 14.7680 23.677 11.838 117.76 0.0 Curvature 1 8.9605 8.9605 8.9605 89.13 0.0 Residual error 5 0.5027 0.5027 0.1005 — — Lack of ﬁt 1 0.0464 0.0464 0.0464 0.41 0.558 Pure error 4 0.4563 0.4563 0.1141 — — Total 8 24.2317 — — — —

Estimated coeﬃcients for avg. US using data in uncoded units

Term Coef.

Constant 611.11

rpm −0.057

s/mm −163.52

related to the lack of ﬁt is very high, since the adopted design cannot allow second-order estimate eﬀects being signiﬁcant in this case.

As for the nugget zone, a 22 factorial design with two centre points and three repeated measurements was carried out for the elongation. Experimental data of yield strength are shown in Table 8.

In this case, a simple ANOVA was carried out since the analysis of variability did not show any signiﬁcant eﬀect. Reliance on this consideration would deem the weights negligible. The ANOVA related to the experimental data of elongation is shown in Table 9.

*The analysis shows a curvature p value of 0.070 that*
*proves its presence; the main eﬀect p value is 0.051; *
*spe-ciﬁcally, the p value related to rpm is 0.037 which is *
*sig-niﬁcant. The p value related to TS*−1is 0.198, which is not
signiﬁcant. The residuals can be assumed to be normally
distributed, with null average and constant standard
*de-viation. An important point is that the high p value related to*
the curvature proves even a lack of ﬁt of the regression
model. Looking data of ultimate strength, yield strength, and
elongation relative of the analysis of variance, it can be seen
that the inﬂuence eﬀects are not signiﬁcant.

Regarding the optimization of the response surface
re-lated to the yield strength, which is the main mechanical
property of interest, an algorithm of steepest ascent to the
yield strength response of the nugget zone was proposed.
*Assuming that x*1*� x*2*� · · · � xk*�*0, where i � 1, 2, . . ., k*
identiﬁes the factors and [−1; 0; 1] are the coded variables
identifying the lower, the centre, and the upper level of the
factors, respectively, the algorithm procedure can be
de-scribed according to the following procedure: deﬁning the
step length for one of the process variables and the step
length of the other variables can be deﬁned by using
*equation (1). Finally, turning the step length ∆xi*from the
coded variable into natural variables.

This algorithm can be applied only when the regression model is of the ﬁrst order and does not include interactions. Runs obtained by implementing the aforementioned algo-rithm are shown in Table 10:

*Δxi*�

*βi*

*βjΔxj*

*,* *with i � 1, 2, . . . , k, i ≠ j.* (1)
The results are similar to those expected, and this
as-certainment guarantees the reliability of the previous
analysis. The average of the yield strength has increased from
a value of 363.33 MPa (point: 1377.5 rpm; 0.267 s/mm) to
values of 399.25 MPa (point: 1250 rpm; 0.241 s/mm) and
395.8 MPa (point: 1150 rpm; 0.213 s/mm). The region where
the two last points are set is the optimum region; a new
investigation using a central composite design would have
been necessary to determine the exact position of the yield
strength optimum point. Following the next steps of the
steepest path, the yield strength decreases, which suggests
that the steepest path is leaving from the optimum region. A
similar behaviour is acted also by the ultimate strength, but
steepest yield strength of the nugget zone path is even one of
the improvement directions of yield and ultimate strength of

the heat-aﬀected zone. Seemingly, the mechanical properties of the HAZ improve markedly when the process gets colder and colder.

As for the shear testing, the results showed averaged failure loads, since three specimens were tested for each run. In Table 11, a summary of averaged failure loads is presented.

According to the tensile testing results, the runs cor-responding to the ﬁrst two steepest ascent algorithms show the best performances for yield strength, especially the run (1150 rpm; 0.213 s/mm) which had an averaged failure load of 10125.16 N. Those failures occur always in the nugget zone explaining the correlation between tensile and shear testing. Vickers microhardness measurements, which were carried out from the centre of the welding along the cross section passing through HAZ, TMAZ, and nugget zone, are shown in Figure 4.

The results reveal a switch of the best mechanical
be-haviour zones, from welds showing better hardness
perfor-mances in the nugget zone to welds showing better hardness
performances in the HAZ. Looking at the welds carried out by
setting rpm equal to 1050 and TS−1_{equal to 0.184 s/mm and}
the ones obtained with rpm equal to 1150 and TS−1equal to
0.213 s/mm (Figure 4), the switch in hardness performances
conﬁrms the results already obtained with tensile testing. In
fact, as well as tensile testing has held up when the runs get
very cold (namely, the following runs: rpm � 950;
TS−1�0.155 s/mm, rpm � 1050; TS−1�0.184 s/mm),
im-proved mechanical behaviour in the HAZ exceeds nugget
zone performance. Thus, microhardness testing conﬁrms the
same trend of tensile testing.

Optical investigations included the study of the oxide ﬁlm; this kind of defect, which is a feature for friction stir welding technology, is commonly called hook defect because of its shape. Hook defects must be taken seriously since they represent cross-section thinning, and for this reason, they may explain shear testing results [31]. Hook’s distances are shown in Table 12.

This study does not contain statistical evidence for
hook’s distance and shear tests correlation; in fact, a linear
regression analysis showed a very low coeﬃcient of
*de-termination (R*2�*0.102 and R*2(adj) � 0) and a very high
*ANOVA p value (F � 0.68; p value � 0.44).*

As for the grain size number of the nugget zone, the results are shown in Table 13.

It can be seen a decrease in grain size for runs featured by high heat generation. A regression analysis between grain size estimates and heat index was carried out as proof. Heat index is considered as a measurement of heat

Table 8: Elongation experimental responses.

rpm s/mm El1 El2 El3 Std. El Dim Avg. El 1377.5 0.267 31.5 30.5 32.0 0.764 3 31.333 2222.5 0.267 9.0 9.0 15.0 3.464 3 11.000 1377.5 0.533 23.0 30.5 27.5 3.775 3 27.000 2222.5 0.533 11.5 4.5 9.0 3.547 3 8.333 1800.0 0.400 33.6 25.0 32.0 4.574 3 30.200 1800.0 0.400 26.0 28.0 31.0 2.517 3 28.333

generated during welding, as the higher the index, the higher is the heat generated. It was deﬁned by using the following equation:

HI � rpm

2

(inch/min) × 10000*.* (2)

The coeﬃcient of determination presented a high value
*(R*2�*0.68, R*2(adj) � 0.63), which suggests a good correlation
between the two parameters, as well the analysis of variance as

Table 9: Results of elongation analysis of variance (nugget zone). Estimated eﬀects and coeﬃcients for avg. El (coded units)

Term Eﬀect Coef. SE coef. *T* *p*

Constant — 19.417 0.5612 34.60 0.018
rpm −19.500 −9.750 0.5612 −17.37 0.037
s/mm −3.500 −1.750 0.5612 −3.12 0.198
rpm ∗ s/mm 0.833 0.417 0.5612 0.74 0.593
Ct Pt — 9.850 1.089 9.04 0.070
*S � 0.619324* *R*2�99.82% *R*2(adj) � 99.09%
Analysis of variance for avg. El (coded units)

Source DF Seq. SS Adj. SS Adj. MS *F* *p*

Main eﬀects 2 179.25 149.80 74.90 195.26 0.051 2-Way interactions 1 0.256 0.211 0.211 0.55 0.593 Curvature 1 31.37 31.37 31.37 81.80 0.070 Residual error 1 0.384 0.384 0.384 — — Pure error 1 0.384 0.384 0.84 — — Total 5 211.26 — — — —

Estimated coeﬃcients for avg. El using data in uncoded units

Term Coef. Constant 71.56 rpm −0.026 s/mm −23.51 rpm ∗ s/mm 0.0074 Ct Pt 9.85

Table 10: Yield strength, ultimate strength, and elongation ex-perimental responses performed along the steepest ascent direction (summarized data for nugget and HAZ).

rpm s/mm Avg. YS Avg. US Avg. El

*Nugget*
1250 0.241 399.25 511.8 28.75
1150 0.213 395.8 507.9 26.36
1050 0.184 339.33 453 25.25
950 0.155 368.67 475.6 25.23
*HAZ*
1250 0.241 370 482.3 19.8
1150 0.213 368 474.5 20.17
1050 0.184 386 491 21.4
950 0.155 405.7 506.25 21.45

Table 11: Shear testing results of averaged failure loads. rpm s/mm Shear testing results (N)

950 0.155 7433.596 1050 0.184 7531.358 1150 0.213 10125.16 1250 0.241 8394.355 1377.5 0.533 5708.624 1377.5 0.267 7768.978 1800 0.25 7001.34 2222.5 0.533 6682.956 2222.5 0.267 4074.074 160 155 150 145 140 135 130 –8 –6 –4 –2 0 2 4 6 8

Distance from the weld centre (mm) RPM = 950; s/mm = 0.155

RPM = 1050; s/mm = 0.184 RPM = 1150; s/mm = 0.213

Hardness (HV)

Figure 4: Vickers microhardness measurement results.

Table 12: Minimum hook distances measured on advancing (AS) and retreating (RS). rpm s/mm Loaded AS thickness (mm) Loaded RS thickness (mm) 950 0.155 0.12 0.12 1050 0.184 0.11 0.12 1150 0.213 0.114 0.116 1250 0.241 0.09 0.12 1377.5 0.533 0.074 0.12 1377.5 0.267 0.032 0.12 2222.5 0.533 0.044 0.12 2222.5 0.267 0.08 0.12

proof of a signiﬁcant inﬂuence of the heat index on grain size
*showing a p value of 0.012. In other words, these analyses*
seem to ensure this assertion: “As big is the heat generation as
big is the grain size in the Nugget Zone.” The mechanical
behaviour of the welds is explained by regression analysis
between hardness Vickers tests and grain size. Such an
analysis revealed a lack of correlation between the two
properties, thus disagreeing with the Hall–Petch rule. So, the
causes of the mechanical behaviour should be found in the
diﬀerences of the weld microstructure; i.e., diﬀerent temporal
thermal proﬁles produce diﬀerent precipitate compositions,
where some are more hardened than others [22, 32, 33].

**4. Conclusions**

In this study, a procedure to optimize the mechanical be-haviour of friction stir welded joints was developed. The yield strength was chosen as a factor of interest, and its response was optimized by using a response surface method. This method, which consisted of a central composite design and a subsequent steepest ascent algorithm, provided for optimal yield strength surface. Tensile tests on base metal specimens were conducted with benchmarking measures obtained from processed samples proving the high perfor-mance of FSW technology. The best perforperfor-mances, which were evaluated choosing the minimum value between HAZ and nugget zone ratio for both yield and ultimate strength, were found under these welding conditions: rpm � 1250 and TS−1�0.241 s/mm. Shear testing conﬁrmed the results provided by tensile tests. Hook’s defect was studied, and the grain size of the nugget zone was estimated.

**Data Availability**

The data used to support the ﬁndings of this study are in-cluded within the article.

**Conflicts of Interest**

The authors declare that they have no conﬂicts of interest.

**References**

[1] V. M. Magalhães, C. Leitão, and D. M. Rodrigues, “Friction
*stir welding industrialisation and research status,” Science and*

*Technology of Welding and Joining, vol. 23, no. 5, pp. 400–409,*

2017.

[2] X. Liu, S. Lan, and J. Ni, “Analysis of process parameters eﬀects on friction stir welding of dissimilar aluminum alloy to

*advanced high strength steel,” Materials & Design, vol. 59,*
pp. 50–62, 2014.

[3] R. Nandan, T. Debroy, and H. Bhadeshia, “Recent advances in
friction-stir welding-process, weldment structure and
*prop-erties,” Progress in Materials Science, vol. 53, no. 6, pp. 980–*
1023, 2008.

[4] Y. S. Sato, M. Urata, and H. Kokawa, “Parameters controlling
microstructure and hardness during friction-stir welding of
*precipitation-hardenable aluminum alloy 6063,” *

*Metallurgi-cal and Materials Transactions A, vol. 33, no. 3, pp. 625–635,*

2002.

[5] A. Ali, M. W. Brown, C. A. Rodopoulos, and S. Gardiner, “Characterization of 2024-T351 friction stir welding joints,”

*Journal of Failure Analysis and Prevention, vol. 6, no. 4,*

pp. 83–96, 2006.

[6] M. W. Mahoney, C. G. Rhodes, J. G. Flintoﬀ, W. H. Bingel,
and R. A. Spurling, “Properties of friction-stir-welded 7075
*T651 aluminum,” Metallurgical and Materials Transactions A,*
vol. 29, no. 7, pp. 1955–1964, 1998.

[7] R. Nandan, G. G. Roy, T. J. Lienert, and T. Debroy,
“Three-dimensional heat and material ﬂow during friction stir
*welding of mild steel,” Acta Materialia, vol. 55, no. 3,*
pp. 883–895, 2007.

[8] H. J. Liu, H. Fujii, M. Maeda, and K. Nogi, “Tensile properties
and fracture locations of friction-stir-welded joints of
*2017-T351 aluminum alloy,” Journal of Materials Processing*

*Technology, vol. 142, no. 3, pp. 692–696, 2003.*

[9] R. F. Gunst, “Response surface methodology: process and
*product optimization using designed experiments,” *

*Techno-metrics, vol. 38, no. 3, pp. 284–286, 1996.*

[10] J. Antony, “Simultaneous optimisation of multiple quality
characteristics in manufacturing processes using taguchi’s
*quality loss function,” International Journal of Advanced*

*Manufacturing Technology, vol. 17, no. 2, pp. 134–138, 2001.*

[11] T. V. Sibalija and V. D. Majstorovic, “An integrated approach
to optimise parameter design of multi-response processes
*based on Taguchi method and artiﬁcial intelligence,” Journal*

*of Intelligent Manufacturing, vol. 23, no. 5, pp. 1511–1528,*

2010.

[12] M. J. Anderson, “A new method for non-parametric
*multi-variate analysis of variance,” Austral Ecology, vol. 26, no. 1,*
pp. 32–46, 2001.

[13] W. B. Schaufeli, M. Salanova, V. Gonz´alez-rom´a, and
A. B. Bakker, “The measurement of engagement and burnout:
*a two sample conﬁrmatory factor analytic approach,” Journal*

*of Happiness Studies, vol. 3, no. 1, pp. 71–92, 2002.*

[14] N. Alagumurthi, K. Palaniradja, and V. Soundararajan,
“Optimization of grinding process through design of
exper-iment (DOE)-a comparative study,” *Materials* *and*
*Manufacturing Processes, vol. 21, no. 1, pp. 19–21, 2006.*

[15] W. Chen, J. K. Allen, K.-L. Tsui, and F. Mistree, “A procedure
for robust design: minimizing variations caused by noise
*factors and control factors,” Journal of Mechanical Design,*
vol. 118, no. 4, p. 478, 1996.

[16] G. Vicente, A. Coteron, M. Martinez, and J. Aracil,
“Appli-cation of the factorial design of experiments and response
*surface methodology to optimize biodiesel production,” *

*In-dustrial Crops and Products, vol. 8, no. 1, pp. 29–35, 1998.*

[17] B. K. Rout and R. K. Mittal, “Parametric design optimization
of 2-DOF R-R planar manipulator-A design of experiment
*approach,” Robotics and Computer-Integrated Manufacturing,*
vol. 24, no. 2, pp. 239–248, 2008.

Table 13: ASTM grains size number versus heat index regression.

rpm s/mm *G* HI
950 0.155 8.54 5.710
1050 0.184 8.60 8.350
1150 0.213 8.66 11.664
1250 0.241 8.72 15.749
1377.5 0.267 8.78 42.841
1377.5 0.533 8.84 21.421
1800 0.25 8.90 54.864
2222.5 0.267 8.96 55.762

[18] A. E. Bryson and W. F. Denham, “A steepest-ascent method
*for solving optimum programming problems,” Journal of*

*Applied Mechanics, vol. 29, no. 2, p. 247, 1962.*

[19] M. Jones, P. Heurtier, C. Desrayaud, F. Montheillet,
D. Allehaux, and J. Driver, “Correlation between
micro-structure and microhardness in a friction stir welded 2024
*aluminium alloy,” Scripta Materialia, vol. 52, no. 8,*
pp. 693–697, 2005.

[20] G. Liu, L. E. Murr, C.-S. Niou, J. C. McClure, and F. R. Vega,
“Microstructural aspects of the friction-stir welding of
*6061-T6 aluminum,” Scripta Materialia, vol. 37, no. 3, pp. 355–361,*
1997.

[21] G. D’Urso and C. Giardini, “The inﬂuence of process
pa-rameters and tool geometry on mechanical properties of
*friction stir welded aluminum lap joints,” International*

*Journal of Material Forming, vol. 3, no. 1, pp. 1011–1014,*

2010.

[22] Y. S. Sato, M. Urata, H. Kokawa, and K. Ikeda, “Hall-Petch
relationship in friction stir welds of equal channel
*angular-pressed aluminium alloys,” Materials Science and Engineering:*

*A, vol. 354, no. 1-2, pp. 298–305, 2003.*

[23] P. M. G. P. Moreira, T. Santos, S. M. O. Tavares, V.
Richter-Trummer, P. Vilaça, and P. M. S. T. de Castro, “Mechanical
and metallurgical characterization of friction stir welding
*joints of AA6061-T6 with AA6082-T6,” Materials & Design,*
vol. 30, no. 1, pp. 180–187, 2009.

[24] L. Commin, M. Dumont, J.-E. Masse, and L. Barrallier,
“Friction stir welding of AZ31 magnesium alloy rolled sheets:
*inﬂuence of processing parameters,” Acta Materialia, vol. 57,*
no. 2, pp. 326–334, 2009.

[25] W. Zhang, Y. Shen, Y. Yan, and R. Guo, “Dissimilar friction
stir welding of 6061 Al to T2 pure Cu adopting tooth-shaped
joint conﬁguration: microstructure and mechanical
*proper-ties,” Materials Science and Engineering: A, vol. 690,*
pp. 355–364, 2017.

[26] R. S. Mishra and Z. Y. Ma, “Friction stir welding and
*pro-cessing,” Materials Science and Engineering: R: Reports,*
vol. 50, no. 1-2, pp. 1–78, 2005.

[27] A. Murphy, M. Price, R. Curran, and P. Wang, “Integration of
strength and process modeling of friction-stir-welded fuselage
*panels,” Journal of Aerospace Computing, Information, and*

*Communication, vol. 3, no. 4, pp. 159–176, 2006.*

[28] A. V. Sergueeva, J. Zhou, B. E. Meacham, and D. J. Branagan,
“Gage length and sample size eﬀect on measured properties
*during tensile testing,” Materials Science and Engineering: A,*
vol. 526, no. 1-2, pp. 79–83, 2009.

[29] M. Ahmadi, F. Vahabzadeh, B. Bonakdarpour, E. Mofarrah,
and M. Mehranian, “Application of the central composite
design and response surface methodology to the advanced
treatment of olive oil processing wastewater using Fenton’s
*peroxidation,” Journal of Hazardous Materials, vol. 123,*
no. 1–3, pp. 187–195, 2005.

[30] W. S. Cleveland and S. J. Devlin, “Locally weighted regression:
*an approach to regression analysis by local ﬁtting,” Journal of*

*the American Statistical Association, vol. 83, no. 403,*

pp. 596–610, 1988.

[31] W. Li, J. Li, Z. Zhang, D. Gao, W. Wang, and C. Dong,
“Improving mechanical properties of pinless friction stir spot
*welded joints by eliminating hook defect,” Materials & Design*

*(1980–2015), vol. 62, pp. 247–254, 2014.*

[32] N. Dialami, M. Chiumenti, M. Cervera, and C. Agelet de
Saracibar, “Challenges in thermo-mechanical analysis of
*friction stir welding processes,” Archives of Computational*

*Methods in Engineering, vol. 24, no. 1, pp. 189–225, 2016.*

[33] M. M. Attallah, C. L. Davis, and M. Strangwood,
“Microstructure-microhardness relationships in friction stir
*welded AA5251,” Journal of Materials Science, vol. 42, no. 17,*
pp. 7299–7306, 2007.